Electro Optical Characterisation of Short Wavelength Semiconductor ...
Basic Concepts Eq. 1.19 delivers directly 2L 2πn λ m λ n = m2π; m = 1, 2, 3 · · · = 2L (1.20) from which the longitudinal mode separation in the cavity could be calculated by differentiation and a mode difference of ∆m = −1 to iii ∆λ = λ2 2nL 1 − λ dn n dλ · (1.21) For a small region the dispersion dn can be neglected; further the substitution of an effective dλ refractive index neff for refractive index n yields ∆λ ≈ λ2 · (1.22) 2neffL Eq. 1.18 is the second condition of lasing. It is already known from (Eq. 1.20) that the wavelength of the lasing regime in the cavity is given by λ = 2nL. Substituted in 1.18 m the cos part turns to unity. The threshold gain will be then gth = αi + 1 1 ln 2L r1r2 (1.23) Obviously the threshold gain gth needs to compensate the internal losses αi and the mirror losses expressed in 1 1 ln 2L r1r2 . By electrically pumped laser diodes the gain has an experimentally proved dependency on the amount of injected carriers which is linear for high gain values (50 − 400cm−1 ) and quadratic, else. This was shown for conventional III-V as well as ZnSe laser diodes. In case of ZnSe laser diodes though, the thermal effects could lead to significant deviations [38, 39]. The linear relationship having the nominal current density J = ηij iv and the transparency current J0 v in mind, can be written as g = Γβ (J − J0) , (1.24) where β is a constant called ’gain factor’ with no further physical meaning . Γ is the confinement factor defining the overlap of light with the gain medium . Using Eqs.1.23 and 1.24 yields directly the Eq.1.25 where the threshold current density jth is calculated; jth = J0d + ηi d αi + βηiΓ 1 1 ln · (1.25) 2L r1r2 The dependency of threshold current density on extrinsic parameters like cavity length and reflectivity of the mirrors leaves the option of modification after growth open. iii ∆m = +1 is also possible. Due to the reciprocal proportionality of m and λ this would result a negative ∆λ. iv ηi is the internal quantum efficiency defined as the ratio of injected carriers to emitted photons contribute stimulated emission and d is the thickness of the active region. v also called nominal threshold current density 12 d
1.3 Laser Device Laser Device A semiconductor laser doesn’t look similar to different people. An electrical engineer may think of it as a forward biased p − n junction, while a crystal grower might be interested in the heterostructure. Nevertheless it is possible to roughly imagine a structure which does ”lase”, as a common underlying picture. A semiconductor laser is generally fabricated by growing a p-doped layer on top of an ndoped substrate. With n- and p-dopes, donor and acceptor impurities in the semiconductor are meant. Popular donors in the III-nitride and II-VI lasers are Si and Cl, respectively; the acceptors mainly used are Mg and N. 1.3.1 Heterostructures The first semiconductor lasers were homostructure devices, i.e. each laser was fabricated with only one semiconductor material. The crucial problem with these lasers was the high threshold current densities, even when operated at low temperatures. Neither could they operate cw. Eq. 1.25 shows the strong proportionality of the threshold current density and the active region thickness d, which is the distance a conducting electron travels from ndoped to p-doped region before recombination with a hole occurs. Retaining other factors, reduction of this thickness reduces the threshold current density. The problem is to trap the electrons in the active region in order to increase the chance of recombination while decreasing the thickness. The method generally adopted is the growth of a blocking layer of a material with a higher bandgap energy than the active region. The resulting structure is called single heterostructure if one blocking layer used and double heterostructure if a blocking layer is used on each side of the active region. Using double heterostructures the thickness bandgap energy refractive index n active region barrier layers cladding layers conduction band valence band Figure 1.8: Schematic diagram of the separate confinement heterostructure (SCH) of the active region in III-nitride as well as II-VI based lasers is reduced to 4 nm. The fact that usually for two materials that can form a stable heterostructure, the larger bandgap material has a lower refractive index, leads automatically to an optical waveguiding for the laser field of double heterostructures. The next steps were increasing output power and lowering laser threshold current. For the double heterostructure described, sailing to higher power is a problem. The reason is that both the carriers and the laser modes are confined in the same thin region. It is desirable to keep the carriers in a thin layer to maximise the density, but the radiation field needs to be in a thick layer so that the intensity of the 13
BIBLIOGRAPHY  G. Snider, 1D Poi